Synthesis and crystal structures of novel alkali rare-earth orthoborates K3RE3(BO3)4 (RE = Pr, Nd, Sm‒Lu)
Chen, Pengyun; Murshed, M. Mangir; Gesing, Thorsten M.; Journal of Materials Science 56 (2021) 3639–3652; doi:10.1007/s10853-020-05506-5

data_1559833
_publ_section_title
;
 Synthesis and crystal structures of novel alkali rare-earth orthoborates
 K3RE3(BO3)4 (RE&#x2009;=&#x2009;Pr,&#x00A0;Nd,&#x00A0;Sm--Lu)
;
_journal_issue                   5
_journal_name_full               'Journal of Materials Science'
_journal_page_first              3639
_journal_page_last               3652
_journal_paper_doi               10.1007/s10853-020-05506-5
_journal_volume                  56
_journal_year                    2021
_chemical_formula_sum            'B4 K3 O12 Tm3'
_chemical_formula_weight         859.33
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_atom_sites_solution_hydrogens   .
_audit_creation_method           SHELXL-2018/3
_cell_angle_alpha                90
_cell_angle_beta                 110.4950(10)
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   10.4900(2)
_cell_length_b                   17.3785(4)
_cell_length_c                   13.7941(3)
_cell_measurement_reflns_used    9722
_cell_measurement_temperature    302(2)
_cell_measurement_theta_max      30.57
_cell_measurement_theta_min      2.34
_cell_volume                     2355.50(9)
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_diffrn_ambient_temperature      302(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0549
_diffrn_reflns_av_unetI/netI     0.0188
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       24
_diffrn_reflns_limit_k_min       -24
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            135682
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         30.604
_diffrn_reflns_theta_min         1.964
_exptl_absorpt_coefficient_mu    23.525
_exptl_absorpt_correction_T_max  0.2913
_exptl_absorpt_correction_T_min  0.1037
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'J. Appl. Cryst. 48 (2015) 3-10'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    4.846
_exptl_crystal_description       PRISM
_exptl_crystal_F_000             3040.0
_exptl_crystal_size_max          0.158
_exptl_crystal_size_mid          0.134
_exptl_crystal_size_min          0.096
_refine_diff_density_max         1.858
_refine_diff_density_min         -1.368
_refine_diff_density_rms         0.211
_refine_ls_extinction_coef       0.000632(10)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2018/3 (Sheldrick 2018)'
_refine_ls_goodness_of_fit_ref   1.109
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     398
_refine_ls_number_reflns         7232
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.109
_refine_ls_R_factor_all          0.0266
_refine_ls_R_factor_gt           0.0191
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0096P)^2^+8.9860P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0341
_refine_ls_wR_factor_ref         0.0356
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                6369
_reflns_number_total             7232
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            K3Tm3BO34-singlecrystal-forCOD.cif
_cod_data_source_block           20200805KTm_0m_a
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_exptl_absorpt_correction_type' value 'Numerical' was
changed to 'numerical' in accordance with the built-in table derived
from the CIF Core dictionary named 'cif_core.dic' version 2.4.5 last
updated on 2014-11-21.

Automatic conversion script
Id: cif_fix_values 8369 2020-08-20 11:38:08Z andrius 
;
_cod_original_sg_symbol_H-M      'P 21/c'
_cod_database_code               1559833
_shelx_shelxl_version_number     2018/3
_shelx_res_checksum              43063